GLOW DISCHARGE SPECTROMETRIES FOR ULTRA FAST DEPTH
PROFILE CHARACTERIZATION OF MATERIALS
P.CHAPON*, S.LEGENDRE, A.TEMPEZ AND C.OLIVERO
HORIBA Jobin Yvon, rue du canal, 91165 Longjumeau Cedex, France
Glow Discharge Spectrometries provide direct
measurement of the chemical composition of
solid materials as a function of depth, with
nanometre resolution and the capability to
measure both thin and thick layers.
All elements can be simultaneously measured
(including H, C, O, Na, Li etc). Deuterium can
be measured with OES, all isotopes being
possible with TOFMS.
The speed of analysis is a key characteristic of
the GD techniques.
These techniques rely on the fast sputtering of a
representative area of the material of interest by a
high density (1014/cm3) and low energy GD
plasma. The same GD plasma assures the
excitation/ionisation of the sputtered species that
are detected in real time by the spectrometer
proving compositional depth profile analysis.
When a high resolution optical system is used,
the resulting technique is called Pulsed RF
GDOES, when the plasma is coupled to ToF MS
detection, it is named Plasma Profiling Time of
Flight Ion Mass Spectrometry.
Various applications are presented and aspects of
analytical performance with regards to
sensitivity, depth resolution, quantification,
repeatability and sample throughput are
Figure 2: Schematic view of the GD plasma
The first illustrative example is taken from the
Photo-Voltaic domain and shows a typical GD
result on a CIGS layer. The crater diameter is
4mm, the total analysis time is 3 minutes.
Figure 1: GD OES analysis of a PV solar cell
The GD plasma source consists in a cylindrical
electrode (typically 4 mm diameter) at ground
potential and the sample powered with a radio
frequency (RF) voltage. The sample placed on an
O-ring is actually “closing” the plasma chamber.
With this geometry, no sample preparation is
needed and starting analysis is almost immediate
upon pumping the vessel to primary vacuum and
letting ultra high purity argon in at a constant
pressure of few mbars. RF excitation is brought
from the back of the sample by means of a
cooled applicator pressing down the sample
against the O-ring. The RF power is supplied by
a 13.56 MHz generator equipped with an
automatic matching network. Sputtered species
induced from Ar ions and fast neutrals
bombarding the sample surface are then excited
The unique characteristics of this plasma allow
very fast erosion (2-10nm/s) with minimum
surface damage (as the incident particles have an
average energy of about 50eV) and it has been
shown that it can be used advantageously for
JP20080241569 and Ref ).
The following example was shown by K.
Shimizu at the 6th International GD day. Sample
is a stainless steel with small inclusions
embedded. The GD plasma allows sputtering the
material down to the inclusions for further SEM
observation and topographic information is
obtained depending on the various nature of the
Figure 3 (a&b): Sputtering of a stainless steel
revealing the grain structure. Zoom on an
embedded inclusion: the GD plasma is revealing
topographic information linked to compositional
changes in the different parts of the inclusion.
2. PULSED RF
A recent development has been the introduction
of Pulsed RF sources offering the capability of
automatic matching in pulsed mode (patent FR
Pulsed RF operation is crucial to avoid unwanted
diffusion of the elements during the
measurements, such as Na in glasses or PV cells.
Enhanced depth resolution is also possible with
The following example with sub-nanometre
depth resolution is taken from [Ref 2] and shows
the Pulsed RF GD OES depth profile of a mirror
Figure 4: Depth profile analysis of a multilayered
Figure 6: Schematic diagram of the TOFMS
instrument (the extraction of the ions is
orthogonal to their direction from the GD source)
The depth resolution is however material
dependant and issues on roughness notably are
Pulsed RF has been crucial also for the
measurement of fragile materials such as
electrodes for Li batteries.
Figure 7: Temporal response of the ion signals
within a GD pulse
Temporal windows in the RF period of the ion
signals for the pre-peak, plateau and/or afterglow
region can be integrated to generate depth
profiles. This unique time resolved information
is highly valuable as it allows for selecting the
higher intensity time window which permits to
gain in sensitivity but also to perform dedicated
studies of plasma/surface interactions.
Figure 5: Depth profile analysis of an electrode
of Li battery with SOC 0% and 100%
When TOFMS detection is used in orthogonal
configuration (cf Figure 6) and at a high
extraction frequency the monitoring of the
temporal ion response from the plasma during
and after the period of the RF pulse is observed.
Details on the different ionisation mechanisms
taking place at the different time domains
(shown in Figure 7) are discussed in [Ref 3].
In other words entire TOF spectra are recorded at
any depth but also virtually at any point during
the RF period.
Figure 8: TOF analytical screen featuring a depth
profile (bottom right), the pulse profile (bottom
left) and the full mass spectrum at selected depth
and time domain in the pulse period.
Plasma gas mixings are commonly used in
plasma deposition but more rarely in analytical
The addition of Oxygen to the plasma gas was
reported to have an adverse effect in GD because
only metallic layers were tried but when
polymeric layers are investigated the use of a
plasma with ArO gas mixing induces chemical
reactions on the surface that complement the
sputtering by the Ar ions and help to dissociate
the chemical bonds of the organic layer.
This new development (patented, FR 50829322)
has opened multiple applications. The following
example is a plastic DVD where nanometre
resolution is obtained on embedded layers below
70 microns of polymer!
Figure 9: Depth profile measurement of a DVD
 Shimizu K., Mitani T.
New Horizons of Applied Scanning Electron
Microscopy, Springer 2010
 Ber B., Bábor P., Brunkov P. N., Chapon P.,
Drozdov M.N., Duda R., Kazantsev D.
Polkovnikov V.N., Yunin P., Tolstogouzov A.,
Thin Solid Films 540 (2013) 96–105
 Mass Spectrometry Handbook,
Chapter 41, Analysis of Thin and Thick Films
Wiley, M.S Lee editor, 2012